**Computational Modeling of Tensile Stress Effects on**

**the Structure and Stability of Prototypical Covalent**

**and Layered Materials**

**Hocine Chorfi1,2, Álvaro Lobato1,3, Fahima Boudjada2,4, Miguel Ángel Salvadó1, Ruth Franco1,**
**Valentín G. Baonza3,5, and J. Manuel Recio1,∗**

1 _{MALTA-Consolider Team and Departamento de Química Física y Analítica, Universidad de Oviedo,}
E-33006 Oviedo, Spain

2 _{University of Constantine, Physics Department, Constantine, Algeria}

3 _{MALTA-Consolider Team and Departamento de Química Física, Universidad Complutense de Madrid,}

E-28040 Madrid, Spain

4 _{Université Claude Bernard Lyon 1, CNRS, Institut Lumiere Matiere, F-69622, Villeurbanne, France}
5 _{Instituto de Geociencias, IGEO, CSIC-UCM, E-28040 Madrid, Spain}

***** Correspondence: jmrecio@uniovi.es; Tel.: +34-985-103036
‡ These authors contributed equally to this work.

**Abstract:** Understanding the stability limit of crystalline materials under variable tensile stress
conditions is of capital interest for their technological applications. In this study, we present results
from first-principles density functional theory calculations that quantitatively account for the response
of selected covalent and layered materials to general stress conditions. In particular, we have
evaluated the ideal strength along the main crystallographic directions of 3C and 2H polytypes of
SiC, hexagonal ABA stacking of graphite and 2H-MoS2. Transverse superimposed stress on the

tensile stress was taken into account in order to evaluate how the critical strength is affected by these multi-load conditions. In general, increasing transverse stress from negative to positive values leads to the expected decreasing of the critical strength. Few exceptions found in the compressive stress region correlate with the trends in the density of bonds along the directions with the unexpected behavior. In addition, we propose a modified spinodal equation of state able to accurately describe the calculated stress-strain curves. This analytical function is of general use and can also be applied to experimental data anticipating critical strengths and strains values and providing informattion on the energy stored in tensile stress processes.

**Keywords:**Ideal strength; quantum-mechanical calculations; SiC; graphite; molybdenum disulfide;
spinodal equation of state.

**1. Introduction**

A clear understanding of cohesive and mechanical properties of technological materials is of capital importance especially when applications are demanded in hostile thermal, stress and chemical environments. Since the nature of the crystalline bonding networks is the ultimate responsible for the response of the compounds to these external conditions, it is rewarding and necessary investigating how macroscopic properties correlate with the chemical interactions at an atomic level. Covalent and layered solids constitute two crystal families currently displaying interest in a variety of areas such as electronics and solar cell industries [1–3]. These compounds provide a good target to examine how changes in strong and weak interactions affect the observed elastic stability of materials. To this end, computer simulations constitute a practical research route to microscopically analyze strained structures of solids since geometries optimized by minimizing the crystal energy can be accurately obtained from first-principles electronic structure calculations under different stress conditions (see for example, Ref. [4]).

Within the above two families of compounds, silicon carbide (SiC), graphite and molybdenum disulfide (MoS2) are pertinent examples because, besides their genuine bonding networks, they

are materials with a variety of applications in several technological sectors as new semiconductor devices, field effect transistors [1,2,5–8], lubricants [9,10] and components of solar cell panels [3]. In the manufacturing processes of these materials, mechanical failure may occur as a result of the stresses induced during the heating cycles to which the compounds are subjected. In addition, the simultaneous existence of covalent and van der Waals interactions leads to preferential bi-dimensional and three-dimensional atomic arrangements in their crystalline structures that result in a high anisotropic response of these materials under variable stress conditions which is worth to be explored.

The challenge consists in the accurate calculation of the limiting tension that these materials can
support in particular directions. Considering perfect non-defective crystals, this maximum tension
is known as the ideal or critical strength (*σ*c) of the material for that direction. Both, experimentally

and theoretically, the evaluation of strain-stress curves constitutes the usual strategy to access to this quantity since after this critical point a catastrophic scenario emerges in form of a crystal fracture or a phase transition. It seems then required to understand how the atomic level interactions correlate with the mechanism of failure in these environmental conditions and, if possible, anticipate the onset of the catastrophic scenario.

A number of theoretical studies using first-principles calculations, mainly employing density functional theory (DFT) [11,12], have permitted a quantitative evaluation of the ideal strength of various materials (see [13,14] and references therein to cite a few) showing that the effect of multi-axial stress obviously depends on the atomic species involved [15,16]. However, to the best of our knowledge, none of these studies have addressed the description of the observed or calculated stress-strain data by means of analytical functions as normally happens for example in high-pressure and related fields. Such equations of state would open the possibility of anticipating critical values for the strength and strain of materials without reaching the instability condition. At this regard, it is pertinent to recall the spinodal equation of state (SEOS) [17]. This analytical function was designed to describe the high-pressure behavior of condensed matter using as a reference state the onset of the elastic instability. It has been successfully applied not only to the description of experimental and theoretical pressure-volume data, but also to the pressure evolution of one dimensional unit cell parameters [18]. Along with this fact, the SEOS is particularly well suited for the description of both experimental and theoretical stress-strain data derived from variable stress tensile conditions since, in the limit, these conditions precisely lead to the elastic instability of the material,i. e., the reference state for this analytical EOS.

In this study, we performed DFT calculations to obtain the ideal strength of 3C and and 2H polytypes of SiC, graphite and 2H-MoS2along their main crystallographic directions without and with

superimposed transverse stress conditions. Results are analyzed in terms of the density of chemical bonds and atomic interactions in the investigated directions of these materials. We are particularly interested in general analytical functions able to represent the behavior of different types of compounds under these tensile conditions and to reproduce the critical parameters. For this end, we propose a new SEOS-form that uses the critical strain as the reference state and that can be easily used to fit both, experimental and calculated stress-strain data.

**2. Computational Details**

2.1. Electronic Structure Calculations

First-principles electronic energy calculations and geometry optimizations under the Kohn-Sham DFT framework of 3C and 2H polytype structures of SiC, ABA stacking of graphite and hexagonal 2H-MoS2 are carried out with the ABINIT code [19,20] using the Perdew-Burke-Ernzerhof (PBE)

exchange-correlation functional [21]. In order to take into account van der Waals forces, the correction (DFT-D2) to the exchange-correlation term, as proposed by Grimme [22], is used for graphite and MoS2. The so-called FHI atomic plane wave pseudopotentials [23] are adopted, while cut off

energies and Monkhorst-Pack grids [24] are set to 1000 eV and 6×6×6 and 6×6×4 for 3C-SiC and 2H-SiC respectively, 1200 eV and 6×6×3 for graphite and 400 eV and 6×6×2 for 2H-MoS2.

Atomic positions are optimized until the total energy converged within 0.1 meV. At the same time, all the strain components (except in the applied loading direction) were optimized so that the corresponding stress components turned out to be within 100 MPa from a predetermined value. The Broyden-Fletcher-Goldfarb-Shanno minimization scheme (BFGS) [20] was used. In this way, tensile-strain curves under controlled normal stress were obtained. Critical strength (ideal strength) was determined as the maximum value of tensile stress before the lattice loses stability and the forces diverge. Multi-axial stress calculations have been performed superimposing a transverse stress to the chosen stress direction. Atomic positions and movements through the different paths are analyzed using the visualization program for structural models (VESTA code) [25].

For the cubic 3C-SiC polytype, we calculate how the stress increases along the [100], [110] and [111] symmetry directions. For the hexagonal 2H-SiC polytype, and graphite and 2H-MoS2layered

crystals, calculations were performed along the inter-plane direction ([001]) perpendicular to the layers, and two in-plane directions, one containing nearest neighbors ([120], so-called zigzag direction) and the other connecting next nearest neighbors ([100], so-called armchair direction).

The stress tensor is calculated in ABINIT as the derivative of the total energy with respect to the
strain tensor. The strain tensor,*e*, can be calculated from the relation between the strain-free lattice

vector of a given atom*µ*,r~*µ*, and its strained lattice vector,r~*µ*0, as follows [26]:

r0*α*

*µ* =r*αµ*+
3

### ∑

*β=1*

*e _{αβ}*r

*, (1)*

_{µ}βwhere*α*and*β*symbols denote the Cartesian components.

In the calculation of the second-order elastic constants in these cubic and hexagonal lattices, we follow an energy-strain scheme (see Refs. [27,28]). The lattice was first relaxed to achieve a zero stress state and then strains were applied by multiplying the lattice vectors by the strain matrix. For a lattice initially under no stress, and using Voigt notation, the energy of the strained lattice can be expressed around the equilibrium position as:

E=E0+

V0

2

### ∑

_{i,j}Cij

*e*i

*e*j, (2)

whereE0andV0are, respectively, the energy and the volume of the unstrained lattice. There are three

independent elastic constants for the cubic lattice (C11,C12,C44) and five independent elastic constants

(C11,C12,C33,C13,C44) for the hexagonal one, thus three and five sets of finite strains were applied

respectively. For each case, eleven equally-spaced strain values were applied between -0.05 and 0.05. The elastic constants were obtained from fitting a quadratic equation to the energy-strain calculated data points. The bulk modulusB0for each structure was calculated using its relationship with the

2.2. Spinodal-like stress-strain equation of state

From a thermodynamic point of view, the elastic stability limit of a solid at athermal conditions is defined by the point where the second derivative of the internal energy with respect to the volume becomes zero. At the corresponding pressure, also named as the spinodal pressure (psp), the bulk

modulus (B) of the substance tends to zero, and therefore any restoring force given by the chemical bonds is overcome, leading to a crystal rupture or a phase transition [29].

The spinodal locus has been considered as an excellent reference to describe the thermodynamic behavior of solids under high pressure conditions [17,30]. Polymers, metals, covalent and ionic crystals have been analyzed showing that theirp-Vdata is accurately and universally represented through the spinodal constrain. This follows from the fact that along a given isotherm, the isothermal bulk modulus depends on the pressure through the following universal relation [31,32]:

B=B?(p−psp)*β*, (3)

whereB?and*β*are, respectively, the amplitude and the pseudocritical exponent that characterize the

pressure behavior of the isothermal bulk modulus.

The spinodal equation of state has not been used only in its volumetric form. For instance, Franciscoet al. [18] studied the evolution under isotropic compression of the lattice parameters of rutile TiO2, showing that a one dimensional (1D) spinodal equation of state (1D-SEOS) can reproduce

accurately their pressure dependence. To that, the authors define a linear bulk modulus, or equivalently
a directional Young modulus (YI, I specifies the direction), and applied the universal relation of Eq.
3. Considering both the physical significance and the directional behaviour of this spinodal-like
equation of state, in this article we introduce a 1D-SEOS to analytically describe the stress-strain curves
associated with tensile stress phenomena. Indeed, under directional stretching, the critical strength
attained along the stress-strain curve corresponds to the spinodal stress limit,*σsp*. The later parameter

accounts for the maximum engineering stress at which the solid breaks, and therefore, represents the elastic limit of the material. Furthermore, at this spinodal point the directional Young modulusYIhas

a value of zero, pointing out that there is no material resistance to a phase transition or rupture. Notice
that these two parameters (*σsp*andYI) are also the one-dimensional analogs of the spinodal pressure

and the bulk modulus. Consequently, from this perspective, the spinodal constrain is clearly fulfilled. Accordingly, the stress dependence ofYIcan be accurately described with an amplitude factorYI?and

a pseudocritical exponent*γ*following an equivalent power law form as Eq.3, and taking into account

the engeneering convention of signs (*σ*is positive for tensile and negative for compressive stress):

YI=YI?(*σ*sp−*σ*)*γ*. (4)

Under these premises, an analytical stress-strain EOS can be derived. As the Young modulus is thermodynamically defined as the derivative of the stress with respect to the strain, the simple integration of Eq.4leads to the following expression for a directional tensile curve:

*σ*=*σsp*− {Y_{I}?(1−*γ*)(*esp*−*e*)}1/(1−*γ)*. (5)

Eq. 5provides an analytical relationship between the stress and the strain along a particular
direction of a crystalline solid involving four characteristic parameters. However, it must be
emphasized that only three are independent since the spinodal strength, the spinodal strain and
the amplitude factor are related realizing that no strain is present at*σ*= 0:

YI?(1−*γ*) =
*σ*sp(1−*γ)*

*e*sp . (6)

*σ*=*σsp* 1−

*esp*−*e*

*e*sp

_{1}_{−}1* _{γ}*!

. (7)

An interesting feature of the proposed stress-strain SEOS is that it can be also expressed analytically in its energy form. In fact, considering the isotherm at 0 K and neglecting zero point vibrational contributions, the stress is related to the internal energyEand the zero-pressure volumeV0

by means of [33]:

*σ*= 1

V0

dE

d*e*. (8)

Consequently, the integrated energy-strain SEOS is:

Esp−E=V0σsp(*esp*−*e*)−V0(1

−*γ*)

(2−*γ*)

*σsp*

*esp*
1
1−*γ*

(*esp*−*e*)

2−*γ*

1−*γ*, (9)

where Esp is the internal energy of the solid at the spinodal strain, or equivalently the spinodal

energy. This quantity must be understood as the energy needed to separate the crystallographic planes perpendicular to the stress-strain direction, and therefore to overcome the interatomic forces. Moreover, the spinodal energy can be expressed in terms of the spinodal stress and spinodal strain once we set to zero the internal energy at zero strain:

Esp=V0*esp*

*σsp*−1−*γ*

2−*γ*

. (10)

An important feature of our current spinodal stress-strain EOS is that the spinodal energy give us the opportunity to connect the mechanical parameters along a given tensile direction with the cohesive interatomic interactions.

Some words of caution on the notation should be given. First,*σc* and*σsp* both represent the

critical or ideal strength of the material along a given direction. The first symbol is obtained from
(*e*i,*σ*i) calculated or experimental data, whereas the second one comes from our 1D-SEOS fittings as

we discuss later. The same applies to*e*cand*e*sp. Second, in our static simulations (zero temperature

and zero point energy contributions neglected), the internal energy of the systemEis reduced to the electronic energy obtained in our DFT calculations. Finally, this symbolEis often used in other works to design the Young modulus. To avoid confussion, here we have chosenYIfor the directional Young

modulus.

2.3. Spinodal Equation of State Fittings

The versatility of the proposed 1D-SEOS allows us fitting Young modulus-stress (Eq. 4),
stress-strain (Eq. 7), and energy-strain (Eq. 10) data. Since the spinodal hypothesis is based on
the assumption that the universal relationship given in expression Eq.3can accurately describe stress
dependence of the directional Young modulus, it becomes first necessary to examine if the proposed
power law can fit in a reliable manner the calculated data. To minimize numerical errors induced
by the second strain derivative of the energy involved in theYI−*σ*curves, a linear interpolation of

the computed electronic energy has been performed. In all the cases, adjusted R-squares for theYI-*σ*

Material Direction *γ* *e*sp *σ*sp

3C-SiC

[100] 0.29 0.35 90.5 [110] 0.49 0.30 52.3 [111] 0.36 0.15 45.1

2H-SiC

[001] 0.36 0.15 44.9 [100] 0.46 0.29 58.0 [120] 0.34 0.17 50.7

Graphite

[001] 0.35 0.99 0.06 [100] 0.53 0.26 85.8 [120] 0.37 0.11 78.3

2H-MoS2

[001] 0.39 0.05 0.07 [100] 0.38 0.27 21.4 [120] 0.46 0.20 14.2

**Table 1.**1D-SEOS parameters from the fittings to our computed stress-strain data. Units of*σ*spare GPa.

As we can see in Table1,*γ*parameter lies inside the 0.41±0.12 interval, depending on the crystal

and the direction considered. These*γ* values are much lower than the universal *β*value of 0.85

assumed by Baonzaet al.for the volumetric compression of solids [17]. Such a difference is attributed to the fact that here we are in the stretching region. Indeed, Broshet al.[34] studied the dependence of the pseudocritical exponent as a function of the reduced volume both in the compressive and expansive regimens. These authors conclude that while the universal pseudocritical exponent of 0.85 accurately describes the solid under high and moderate pressure, the exponent goes down to the value of 0.5 in the case of the negative pressure regime, which is within the range of the results obtained in our spinodal stress-strain equation of state.

**3. 3C-SiC, 2H-SiC, Graphite and 2H-MoS**2**: Results and Discussion**

3.1. Bulk Properties

**Table 2.**Zero pressure lattice and elastic constants of 3C- and 2H-SiC polytypes, graphite and 2H-MoS2.
AllB0values calculated using Voigt elastic constants relationship.

This work Calculated Experimental

3C-SiC

a(Å) 4.39 4.34 [35], 4.38 [36] 4.34 [37]

C11(GPa) 341 390 [35], 385 [36] 352 [38]

C12(GPa) 130 134 [35], 128 [36] 140 [38]

C44(GPa) 224 253 [35], 264 [36] 233 [38]

B0(GPa) 200 219, 213 211

2H-SiC

a(Å) 3.085 3.05 [39], 3.09 [36] 3.076[40]

c(Å) 5.060 5.00 [39], 5.07 [36] 5.224 [40]

C11(GPa) 528 541 [39], 536 [36] 501±4 [41]

C12(GPa) 112 117 [39], 78 [36] 111±5 [41]

C33(GPa) 565 586 [39], 573 [36] 553±4 [41]

C13(GPa) 52 61 [39], 31 [36] 52±9 [41]

C44(GPa) 156 162 [39], 164 [36] 163±4 [41]

B0(GPa) 228 238, 214 220

Graphite

a(Å) 2.521 2.451 [42] 2.464 [43]

c(Å) 7.067 6.582 [44] 6.712 [43]

C11(GPa) 892 1118 [45] 1109±16 [43]

C12(GPa) 163 235 [45] 139±36 [43]

C33(GPa) 31 29 [45] 38.7±7 [43]

C13(GPa) 5 8.5 [45] 0±3 [43]

C44(GPa) 6 -2.8 [45] 5±3 [43]

B0(GPa) 240 307 281

2H-MoS2

a(Å) 3.19 3.16 [46] 3.163 [47]

c(Å) 12.56 12.296 [46] 12.341 [47]

C11(GPa) 220 218 [46] 238 [48]

C12(GPa) 45 38 [46] -54 [48]

C33(GPa) 40 35 [46] 52 [48]

C13(GPa) 16 17 [46] 23 [48]

C44(GPa) 26 15 [46] 19 [48]

B0(GPa) 75 68 57

3.2. Ideal strength with and without transverse stress

This subsection is devoted to the calculation of the strain-stress curves of the four structures considered in this study. First, we collect in Fig.1the results under vanishing transverse stress. For 3C-SiC and 2H-SiC, calculated points are very similar to those reported by Umeno, Kubo, and Nagao [36]. For graphite, our in-plane stress-strain curves show maxima at similar strain values to those reported by Liual.[42] for graphene, although we compute critical strengths along these directions around 25 GPa lower than in their work. This is due in part to differences between LDA (Liuet al.) and GGA (ours) levels of calculation, and on the other hand, to differences in the system, single sheet (graphene) and the bulk (graphite). To the best of our knowledge, the corresponding curve for thec direction has not been reported so far. Analogously, we have not found previous strain-stress curves along this direction for bulk 2H-MoS2, whereas for the in-plane directions the previous reported

studies refer to single- or few-layers 2H-MoS2[49,50]. These results indicateg a noticeable decreasing

of*σc*as the size of the slab increases, which is also the expected trend according to our calculations.

effects induced in the chemical bonds by the tensile strain (changes in bonding lengths and angles) are essentially captured in this parameter. EBL values exhibit the expected trend always increasing as the strain increases up to the stability limit.

Fig.1(a) shows that in 3C-SiC the slopes in the low strain region are nearly equal regardless the
direction. However, the maximum stress value strongly depends on the direction of the deformation
with an ideal strength nearly twice larger along the [100] axis (*ec*= 0.35 and*σc*= 91 GPa) as that found

for [110] (*ec*= 0.30 and*σc*=53 GPa) and [111] (*ec*= 0.15 and*σc*= 45 GPa). We notice that along [100] all

tensile forces are equally distributed over the Si-C bonds. This is in contrast to the tension along [110] and [111] directions. For example, in the latter, one of the four C nearest neighbors of a given Si atoms stand along the same [111] direction and the corresponding Si-C bond suffers apurestretching, whereas the stretching of the other three Si-C bonds is not so effective and involves bond angle modifications upon the tensile strain along this [111] direction. At zero strain, the previously defined EBL parameter already has a value roughly twice greater for the [100] direction (17.5 Å) than for the [110] (9.3 Å) and [111] (9.5 Å) directions. Thus, although the order between the [100] and [111] directions is not captured considering just the equilibrium structure, the EBL parameter catches the essential difference between the [100] direction and these two other directions.

The stress-strain curves during uniaxial tension with vanishing transverse stress in 2H-SiC is
shown in Fig.1(b). Slopes in the low strain (harmonic) region are almost exactly equal whereas the
maximum stress value strongly depends on the direction of the deformation. The stress-strain relation
in 2H-SiC [001] (*ec*= 0.15 and*σc*= 45 GPa) and 3C-SiC [111] are nearly identical. It is so because of

the similarity of the lattice planes normal to the stress direction, and so are the curves of 2H-SiC [100]
(*ec*= 0.29 and*σc*= 58 GPa) and 3C-SiC [110]. The stress-strain relation in 2H-SiC along [120] shows

intermediate values (*e*c= 0.20 and*σ*c= 50 GPa). Again, these values correlate with the effective Si-C

bond lengths along the corresponding directions. Calculated EBL values in Å for the [100], [120] and
[001] are, respectively, 21.3, 16.8, and 12.3, following the same trend as*σc*and in agreement also with

previous interpretations in terms of next-nearest Si-C interactions by Umenoet al.[36].

In Fig. 1(c) and (d), the responses of graphite and 2H-MoS2 to tensile stress along the [100],

[120], and [001] directions are displayed. Here, the laminar nature of these two compounds is clearly
revealed by very low ideal strength values along thecaxis (*ec*= 0.13 and*σc*= 0.063 GPa in graphite

and*ec*= 0.05 and*σc*= 0.069 GPa in 2H-MoS2) which is in concordance with the weak van der Waals

nature of the inter-layer interaction. At low strains, the in-plane graphite strains reveal an isotropic 2D
elastic behavior in good agreement with previous DFT calculations [51]. At large in-plane strains, the
lattice layers start to behave anisotropically and the critical stress along the next-nearest-neighbor [100]
direction (*e*c= 0.26 and*σ*c= 86 GPa in graphite and*e*c= 0.27 and*σ*c= 22 GPa in 2H-MoS2) becomes

greater than that along the nearest-neighbor [120] direction (*ec*= 0.11 and*σc*= 78 GPa in graphite

and*ec*= 0.20 and*σc*= 14 GPa in 2H-MoS2). Expected differences between stronger C-C than Mo-S

intralayer bonds are also clearly manifested when comparing these data.

For all directions and structures, we now analyze new results coming from the proposed analytical
1D-SEOS. All the curves in the four panels of Fig.1were obtained from the 1D-SEOS fittings to the
calculated strain-stress data. The performance of the 1D-SEOS is apparent and allows us to derive
with confidence critical stress and critical strain values from the corresponding fitting parameters*σsp*

and*e*sp, respectively. We have checked that the trends and specific values of these two key parameters

compare with high accuracy with our first-principles computed numerical values (see Table1). Thus, we arrive to this interesting conclusion: the 1D-SEOS of Eq.7is an appropriate analytical function for describing stress-strain data.

We have noticed earlier that multi-load conditions may be present in manufacturing processes combining thermal effects and epitaxial growth. As a particular situation of these conditions, we have studied in a second round of simulations the effects of superimposing transverse stress (both compressive and tensile) on the previous tensile directions for the four structures. We detectec convergence problems in some simulations that have hindered the calculations in the compressive (negative) transverse stress range in 2H-MoS2, and also along the [100] direction in the positive range

of this compound. The expected trend is a decreasing of the critical strength as we increase the
superimposed transverse stress from negative to positive values. In fact, this is the computed behavior
for the majority of situations we have studied. For example, the critical strength*σc*is lowered by the

transverse stress*σt*in all the directions in 3C-SiC (except [110]), 2H-SiC (except [100]), graphite, and

2H-MoS2. In this two laminar compounds, we obtain just one value at the most negative transverse

stress breaking the decreasing trend along the [120] direction. All these results are displayed in Fig.2 and are in complete agreement with the computed data in 3C- and 2H-SiC reported by Umenoet al. [36]. In general, the unexpected positive slope in the ideal strength-transverse stress curve appears at compressive transverse stress values. In the tensile regime, all the directions and structures show a modulated lowering of the ideal strength as the transverse tension increases which is compatible with the overall weakening of the compounds as multi-load conditions are enhanced or, in Umenoet al. words, to the higher strain energy stored in the material.

Interestingly enough, we have observed an equivalent behavior when we analyze the computed
EBL parameters. In all but the cases where we have detected an exception, the calculated effective
bond length parameter at the critical strain condition decreases monotonically as we superimpose the
transverse stress on the corresponding tensile strain direction. Thus, we found that the decreasing of
the ideal strength value correlates with the decreasing in the EBL parameter. For example, along the
[111] direction in 3C-SiC, EBL continuously decreases from 11.00 Å at*σt*= -30 GPa to 10.78 Å at*σt*

= +30 GPa. The corresponding values at the same transverse stress conditions for the [100] direction
are 24.71 Å and 21.18 Å. Similar trends are found for the EBL parameter along the [120] and [001]
directions in 2H-SiC. On the contrary, in those cases where negative transverse stresses induce an
unexpected behavior, this EBL parameter also shows an increasing as the transverse stress increases
up to the condition of vanishing transverse stress. Thus, along [110] in 3C-SiC and [100] in 2H-SiC, the
values of EBL at*σ*t= -30 GPa are, respectively, 10.94 Å and 26.08 Å, increasing up to 11.49 Å and 26.24

Å at*σ*t= 0 GPa, and finally decreasing to 10.97 Å and 24.13 Å at*σ*t= +30 GPa. The reason why a

reduction in the critical strength occurs as compressive transverse is superimposed has been explained
by the appearance of a thermodynamic competitive phase as the rock-salt structure in 3C-SiC [36].
Here, we also see that this reduction in the*σ*calso correlates with the fact that the effective Si-C bond

lengths along the [110] and [100] directions in 3C-SiC and 2H-SiC, respectively, show lower values at the critical conditions when the compressed transverse stress is increased, thus correlating with the trend followed by the critical strengthe.

**Figure 2.**Calculated critical stress-transverse stress curves for: (**a**) 3C-SiC, (**b**) 2H-SiC, (**c**) Graphite, and
(**d**) 2H-MoS2.

3.2.1. Other outcomes of the stress-strain SEOS: energetics and directional Young moduli

calculated (*e*i,*σ*i) data points are well described by the proposed 1D-SEOS. Here, the integrated SEOS

for all the directions and materials studied in this work are represented in Fig. 3. The symbols correspond to the energy minima at selected strains obtained from our first-principles calculations. The calculated parameters associated with the integrated forms are collected in Table3.

The analytical energy curves clearly reflect the good quality of the fittings (see Fig. 3). Two
parameters define the shape of each of these curves,*esp*andEsp. The first one, previously discussed in

relation to the stress-strain curves (see Table1), identifies the abscissa of the inflexion point, where the directional Young modulus vanishes. The ordinate of this point isEsp(see Table3) and correlates

quite well with the critical/spinodal strength calculated along each of the directions explored for the
materials under study in this work. The higher the strength, the higher the energy required to induce
an elastic instability in the material. Not surprising, the highest values are obtained in 3C-SiC along
the [100] direction and graphite along the [100] direction, just the same systems and directions where
we had found the greatest values for*σc*(and*σsp*).Espvalues provide also information on the energy

stored in the material due to the tensile stretching. For example, along the last two directions the energy stored is expected to be higher than along other directions with flatter energy-strain curves, as [001] directions in graphite and 2H-MoS2(see Fig. 3). Notice that for these two situations with the

weakest cohesive interactions, values are so low (within the accuracy of the calculations) that only a limit value is given. Overall, we believe that these results evidence the utility of the energy-strain SEOS.

As regards the directional Young modulus, we can easily derive a simple expression at zero stress YI(0) involving the three parameters of the stress-strain 1D-SEOS by evaluating Eq.4at zero stress:

YI(0) =

*σsp*

*esp*(1−*γ*). (11)

This parameter is discussed below.

**Table 3.**Energy and Young modulus parameters from the integrated stress-strain SEOS fittings

Material Direction YI(0)(GPa) Esp(kJ/mol)

3C-SiC

[100] 396 219

[110] 407 110

[111] 478 50

2H-SiC

[001] 481 50

[100] 437 142

[120] 450 66

Graphite

[001] 0.99 <1

[100] 746 201

[120] 746 113

2H-MoS2

[001] 2.41 <1

[100] 150 69

[120] 140 153

In 3C-SiC, the directional Young moduli at zero stress are (in GPa) 396, 406, 478 GPa for the [100] [110] and [111] directions, respectively. These results are in concordance with the directional Young moduli calculated through the theory of representation surfaces [52]. For instance, in the case of the [111] direction

Y111=

S11−

2 3

S11−S12−

1 2S44

−1

, (12)

whereS11,S12, andS44are the compliance constants related to the elastic constants by:

S11= C11

+C12

(C11−C12)(C11+2C12)

,S12=

−C12

(C11−C12)(C11

+2C12),S44= 1

C44

According to the data from Table2, and using the above equations, the calculated value forY111(0) is

489 GPa in good agreement with the parameter obtained from our 1D-SEOS.

In this case, the elastic behavior of the cubic SiC polytype is not enterely isotropic andYI(0) slightly

increases along the sequence [100] [110] and [111].YI(0) provides a quantitative measure of the initial

slope of the stress-strain curve, thus representing the resistance of the material to a tensile distortion along a particular direction at equilibrium. Under this perspective, the values ofYI(0) in the [100],

[110] and [111] series of 3C-SiC inform that the direction [111] offers the highest resistance to a strain stretching at zero stress. In 2H-SiC, the values ofYI(0) point out that all the directions studied present

similar resistance to distortion. Here, the solid behaves less anisotropically than in the case of the cubic polytype, expanding a narrower range of values, although both polytypes display similar zero stress Young moduli.

Let us finally conclude analyzing these zero stress directional Young moduli in graphite and 2H-MoS2. Layered materials constitute a severe test for our model since weak and covalent interactions

are simultaneously present. In both compounds, the van der Waals nature of the inter-layer interactions is revealed through the values of the directional Young modulus provided by the spinodal parameters. Y001(0) values (in GPa) are as low as 0.99 and 2.40 for graphite and 2H-MoS2, respectively, in contrast

with the values along the [100] and [120] directions which are, respectively, 748 and 728 for graphite, and 150 and 140 for 2H-MoS2. The latter values can be compared with the intra-layer Young modulus

reported for graphite and MoS2by other authors. For instance, for graphite goes from 700 to 1100

GPa ([51] and references therein), whereas for 2H-MoS2the values range between 130 and 220 GPa

[53–55] showing a good agreement with the results obtained in this work. At this point, it must also be emphasized that our Young modulus values reflect the expected different intralayer bond strengths between the C-C and Mo-S bonds, as we previously detected in the analysis of the 1D-SEOS parameters (see subsection3.2).

**Figure 3.**Calculated energy-strain curves for: (**a**) 3C-SiC, (**b**) 2H-SiC, (**c**) Graphite, and (**d**) 2H-MoS2.

**4. Conclusions**

The ideal strength of 3C- and 2H-SiC, graphite, and 2H-MoS2were evaluated by means of first

principles quantum-mechanical methodologies based on the DFT approximation. Both, vanishing
and superimposed transverse stress over uniaxial tensile strains were considered in order to evaluate
the ideal strength of the four crystalline structures. The ideal strength is found to depend on the
particular crystallographic direction revealing the expected stronger mechanical anisotropy in the
layered compounds. In graphite and molybdenum disulfide layers, after an isotropic behavior at the
low strain regime, we observe a different behavior along the two in-plane directions, being the ideal
tensile strength smaller in the nearest-neighbor than in the next-nearest-neighbor direction. In these
crystals, the lowest value of*σ*cis obtained in thec-direction as expected given the weak inter-layer vdW

interactions. The ideal tensile strength is generally decreased by the transverse tension. Reduction in the ideal strength by large transverse compression occurs in some structures and orientations in concordance with an increasing on the effective bond lengths in those conditions.

We present a new 1D-SEOS analytical function that was successfully applied to the computed
strain-stress data points, and that can be also used to describe results from tensile stress experiments.
The spinodal strain*esp*along with the corresponding spinodal stress*σsp*fitting parameters have been

**Author Contributions:**Conceptualization, J.M.R., M.A.S., A.L., V.G.B. and F.B.; methodology, C.H., M.A.S. and
A.L.; investigation, C.H., A.L. and R.F.; writing–original draft preparation, C.H., J.M.R. and A.L.; writing–review
and editing, J.M.R.; A. L., R. F.; supervision, V.G.B., J.M.R., F.B. and M.A.S.; project administration, R.F.; funding
acquisition, V.G.B., J.M.R. and M.A.S.

**Funding:** This research was funded by the EU (FEDER) and Spanish institutions MINECO and MICINN
under the projects CTQ2015-67755-C2-R and PGC2018-094814-B-C22, and Principado de Asturias-FICYT, project
GRUPIN14-049.

**Acknowledgments:** Special thanks are due to the colleague A.H. Meziani for useful discussions. Computer
facilities of MALTA-Computer center at the Universidad de Oviedo are gratefully acknowledged.

**Conflicts of Interest:** The funders had no role in the design of the study; in the collection, analyses, or
interpretation of data; in the writing of the manuscript, or in the decision to publish the results.

**References**

1. Asano, K.; Hayashi, T.; Takayama, D.; Sugawara, Y.; Ryu, S.H.; Palmour, J.W. Temperature dependence of
On-state characteristics, and Switching characteristics of 5 kV class 4H-SiC SEJFET.IEEJ Trans. IA**2005**,125
(2), 147-152.

2. Peña-Álvarez, M.; del Corro, E.; Morales-García, Á.; Kavan, L.; Kalbac, M.; Frank, O. Single Layer
Molybdenum Disulfide under Direct Out-of-Plane Compression: Low-Stress Band-Gap Engineering.Nano
Letters**2015**,15, 3139–3146.

3. Tsai, M.-L.; Su, S.-H.; Chang, J.-K.; Tsai, D.-S.; Chen, C.-H.; Wu, C.-I.; Wu, Li, L.-J.; Chen, L.-J.; He, J.-H.
Monolayer MoS2heterojunction solar cells.ACS Nano**2014**,8, 8317–8322.

4. Recio, J.M.; Menéndez, J.M.; Otero-de-la-Roza, A.; Eds.An Introduction to High-Pressure Science and Technology

CRC-Press, Boca Raton, 2016.

5. Radisavljevic, B.; Radenovic, A.; Giacometti, V.; Kis, A. Single-layer MoS2transistors.Nat. Nanotechnol.**2011**,

6, 147-150.

6. Wang, H.; Yu, L.; Lee, Y.H.; Shi, Y.; Hsu, A.; Chin, M.L.; Li, L.J.; Dubey, M. Kong, J.; Palacios, T. Integrated
circuits based on bilayer MoS2transistors.Nano Lett.**2012**,12, 4674-4680.

7. Fiori, G.; Szafranek,B.N.; Iannaccone, G.; Neumaier, D. Velocity saturation in few-layer MoS2transistor.Appl.

Phys. Lett**2013**,103, 233509(1)-233509(4).

8. Kim, S.; Konar, A.; Hwang, W.S.; Lee, J.H.; Yang, J.; Jung, C.; Kim, H.; Yoo, J.B.; Choi, J.Y. High-mobility and
low-power thin-film transistors based on multilayer MoS2crystals.Nat. Commun.**2012**,3, 1011-1017.
9. Bollmann, W.; Spreadborough, J. Action of Graphite as a Lubricant.Nature**1960**,186, 29-30.

10. Peelaers, H.; Van de Walle C. G. Elastic Constants and Pessure-Induced Effects in MoS2.J. Phys. Chem.**2014**,

118, 12073-12076.

11. Kohn, W.; Sham, L.J. Self-Consistent Equations Including Exchange and Correlation Effects.Phys. Rev.**1965**,

140A, 1133-1138.

12. Argaman, N.; Markov, G. Density functional theory: An introduction.Am. J. Phys.**2000**,68(1), 69-79.
13. Umeno, Y.; Kitamura, T. Ab Initio Simulation on Ideal Shear Strength of Silicon.Mater. Sci. Eng.**2002**,B

88-1, 79-84.

14. Cerny, M.; Rehak, P.; Umeno, Y.; Pokluda, J. Stability and strength of covalent crystals under uniaxial and
triaxial loading from first principles.J. Phys. Condens. Matter**2013**,25, 35401-35408.

15. Umeno, Y.; Cerny, M. Effect of normal stress on the ideal shear strength in covalent crystals.Phys. Rev. B

**2008**77, 100101-100104.

16. Umeno, Y.; Cerny, M. Ideal shear strength under compression and tension in C, Si, Ge, and cubic SiC: an ab
initio density functional theory study.J. Phys. Condens. Matter**2011**,23, 385401(1)-385401(7).

17. Baonza, V.G.; Cáceres, M.; Nú nez, J. Universal compressibility behavior of dense phases.Phys. rev. B;**1995**,

51, 28-37.

18. Francisco, E.; Bermejo, M.; García Baonza, V.; Gerward, L.; Recio, J.M. Spinodal equation of state for rutile
TiO2.Phys. Rev. B;**2003**,67, 064110(1)- 064110(8).

20. Gonze, X.; Amadon, B.; Anglade, P.-M.; Beuken, J.-M.; Bottin, F.; Boulanger, P.; Bruneval, F.; Caliste, D.;
Caracas, R.; Côté, M.; Deutsch, T.; Genovese, L.; Ghosez, Ph.; Giantomassi, M.; Goedecker, S.; Hamann, D. R.;
Hermet, P.; Jollet, F.; Jomard, G.; Leroux, S.; Mancini, M.; Mazevet, S.; Oliveira, M. J. T.; Onida, G.; Pouillon,
Y.; Rangel, T.; Rignanese, G.-M.; Sangalli, D.; Shaltaf, R.; Torrent, M.; Verstraete, M. J.; Zerah, G.; Zwanziger, J.
W.ABINIT: First-principles approach to material and nanosystem properties.Comput. Phys. Commun.**2009**,

180, 2582-2615.

21. Perdew, J.P.; Burke, K.; Ernzerhof, M. Generalized Gradient Approximation Made Simple.Phys. Rev. Lett.;
**1996**,77, 3865-3868.

22. Grimme, S. Semiempirical GGA-Type Density Functional Constructed with a Long-Range Dispersion
Correction.J. Comp. Chem.;**2006**,27, 1786-1799.

23. Trouillier, N.; Martins, J.L. Efficient pseudopotentials for plane-wave calculations.Phys. Rev. B;**1991**,43, 3,
1993-2006 .

24. Monkhost, H.J.; Pack, J.D. Special points for Brillouin-zone integrations.Phys. Rev. B;**1976**,13, 5188-5192.
25. Momma, K.; Izumi, F. VESTA 3 for three-dimensional visualization of crystal, volumetric and morphology

data.J. Appl. Crystallogr.;**2011**,44, 1272–1276.

26. Born, M.; Huang, K.Dynamical Theory of Crystal Lattice, Oxford Clarendon Press, London, 1966.

27. Zeina M.J.; Servio, P.; Rey A.D. Ideal Strength of Methane Hydrate and Ice Ih from First-Principles.Cryst.
Growth. Des.;**2015**,15, 5301-5309.

28. Otero de la Roza, A.; Luaña, V. Runwien: a text-based interface for the WIEN package.Computer Physics
Communications;**2009**,180, 800–812.

29. Baonza, V.G.; Taravillo, M.; Cáceres, M.; Núñez, J. Universal features of the equation of state of solids from a
pseudospinodal hypothesisPhys. rev. B;**1996**,53, 5252-5258.

30. Taravillo, M.; Baonza, V.G.; Núñez, J.; Cáceres, M. Simple equation of state for solids under compression.

Phys. rev. B;**1996**,54, 7034-7045.

31. Baonza, V.G.; Cáceres, M.; Núñez, J. High-pressure compressibility behavior of liquids referred to a
pseudospinodal curve.Chem. Phys. Lett.;**1994**,228, 137-143.

32. Baonza, V.G.; Cáceres, M.; Núñez, J. Universal Behavior of Compressed Liquids.J. Chem. Phys.;**1994**,19,
4955-4958.

33. Ogata, S.; Li, J.; Shibutant, N.; Yip, S. Ideal shear strain of metals and ceramics. Phys. Rev. B**2004**,70,
104104(1)-104104(7).

34. Brosh, E.; Makov, G.; Shneck, R.Z. The spinodal constraint on the equation of state of expanded fluids.J.
Phys.: Condens. Matter;**2003**,19, 2991-3001.

35. Karch, K.; Pavone, P.; Windl, W.; Schuelt, O.; Strauch, D. Ab initio calculation of structural and
lattice-dynamical properties of silicon carbide.Phys. Rev. B;**1994**,50, 17054-17063.

36. Umeno, Y.; Kubo, A.; Nagao, S. Density functional theory calculation of ideal strength of SiC and GaN: Effect
of multi-axial stress.Comput. Mater. Sci.;**2015**,109, 105-110.

37. http://www.ioffe.ru/SVA/NSM/(Ioffeinstitut, 2003).

38. Li, Z.; Brandt, R.C. The single-crystal elastic constants of cubic (3C) SiC to 1000◦C.J. Mater. Sci.;**1987**,22,
2557-2559.

39. Saramasak, K.; Limpijumnong, S.; Lambrecht, W.R.L.Comput. Mater. Sci.;**2010**,49, 543-546.

40. Villard, P.; Calvert, L.D.Pearson’s Handbook of Crystallographic Data for intermetallic Phases; ASM international. Cleveland. 1991.

41. Kamitani, K.; Grimsditch, M.; Nipko, J. C.; Loong, C.K.; Okada, M.; Kimura, I. The elastic constants of silicon
carbide: A Brillouin-scattering study of 4H and 6H SiC single crystals.J. Appl. Phys.;**1997**,82, 3152-3154.
42. Liu, F.; Ming, P.; Li, J. Ab initio calculation of ideal strength and phonon instability of graphene under

tension.Phys. Rev. B;**2007**,76, 064120(1)- 064120(7).

43. Bosak, A.; Krisch, M.; Mohr, M.; Maultzsch, J.; Thomsen, C. Elasticity of single-crystalline graphite: Inelastic
x-ray scattering study.Phys. Rev. B;**2007**,75, 153408(1)-153408(4)

44. Ooi, N.; Rairkar, A.; Adams, J.B. Density functional study of graphite bulk and surface properties.Carbon;
**2006**,44, 231-242.

46. Alexiev, V.; Prins, R.; Weber, T. Ab initio study of MoS2and Li adsorbed on the (10-10) face of MoS2.Phys.

Chem. Chem. Phys.;**2000**,2, 1815-1827.

47. Fan, D.; Xu, J.; Ma, N.; Liu, J.; Xie, H. P-V-T Equation of state of molibdenite (MoS2) by a diamond anvil cell
and in situ synchrotron angel-dispersive X-ray diffraction.Physica B;**2014**,451, 53-57.

48. Feldman, J. L. Elastic constants of 2H-MoS2and 2H-NbSe2extracted from measured dispersion curves and
linear compressibilities.J. Phys. Chem. Solids;**1976**,37, 1141-1144.

49. Li, T. Ideal strength and phonon instability in single-layer MoS2.Phys. Rev. B;**2012**,85, 235407(1)-235407(5).
50. Li, P.; Jiang, C.; Xu, S.; Zhuang, Y.; Gao, L.; Hu, A.; Wang, H.; Lu, Y. In situ nanomechanical characterization

of multi-layer MoS2membranes: from intraplanar to interplanar fracture.Nanoscale;**2017**,9, 9119-9128.
51. Abbasi-Pérez, D.; Menéndez, J.M.; Recio, J.M.; Otero-de-la-Roza, A.; del Corro, E.; Taravillo, M.; Baonza,

V.G.; Marqués, M. Modeling graphite under stress: equations of state, vibrational modes, and interlayer
friction.Phys. Rev. B;**2014**,90, 054105(1)-054105(10).

52. Nye, J.F.Physical Properties of Crystals, Oxford Science Publications, U.S.A., 1989.

53. Bertolazzi, S.; Brivio, J.; Kis, A. Stretching and Breaking of Ultrathin MoS2.ACS Nano;**2011**,5, 9703-9709.
54. Lorenz, T.; Teich, D.; Joswig, J.O.; Seifert, G. Theoretical Study of the Mechanical Behavior of Individual TiS2

and MoS2Nanotubes.J. Phys. Chem. C;**2012**,116, 11714-11721.

55. Cooper, R.C.; Lee, C.; Marianetti, C.A.; Wei, X.; Hone, J.; Kysar, J.W. Nonlinear elastic behavior of
two-dimensional molybdenum disulfide.Phys. rev. B;**2013**,87, 035423-1-035423-11.

56. Li, W.; Wang, T. Elasticity, stability, and ideal strength of ß-SiC in plane-wave-based ab initio calculations.

Phys. Rev. B**1999**,59, 3993-4001.

57. Kohyama, M. Tensile strength and fracture of a tilt grain boundary in cubic SiC: a first-principles study.Phil.
Mag. Lett.**1999**,79, 659-672.

58. Martin, J.; Donnet, C. Le Mogne, Th. Epicier, Th. Superlubricity of molybdenum disulphide.Phys. Rev. B

**1993**,48, 10583-10586.

59. Otero de la Roza, A.; Abbasi, D.; Luaña, V. Gibbs2: A new version of the quasiharmonic model code. II.
Models for solid-state thermodynamics, features and implementation.Comput. Phys. Commun.;**2011**,182,
2232-2248.

60. Catti, M. Crystal Elasticity and Inner Strain: a Computational Model.Crystal Elasticity and inner strain: a
computational model, Acta Crystallogr.;**1989**,sect. A 45, 20-25.

61. Kudin, K.N.; Scuseria, G.E.; Yakobson, B.I.C2F, BN, and C nanoshell elasticity from ab initio computations.